1 Metallogr. Microstruct. Anal. (2013) 2: DOI /s TUTORIAL Heat Treating of Nonferrous Alloys Howard E. Boyer Ó American Society for Metals 1984 The reader should understand at the outset that this chapter is intended to present only an overview of the heat treating of nonferrous alloys. First, a brief discussion of the effects of cold work and annealing on nonferrous alloys is presented. This is followed by discussion of the mechanisms involved in the more common heat treating procedures used for hardening or strengthening solution treating and aging. No attempt is made in this treatise to cover the more complex procedures required for duplex structures which characterize some nonferrous alloys, notably titanium and copper alloys. For more complete information on the heat treating of nonferrous alloys and the properties that may be obtained, see Metals Handbook, Vol 4, 9th edition, American Society for Metals, 1981, and Heat Treatment, Structure and Properties of Nonferrous Alloys, by Charlie R. Brooks, American Society for Metals, Work Hardening Most metals and metal alloys (ferrous and nonferrous) respond to hardening from cold work. There is, however, a wide variation among the many metal and metal alloy combinations in their rate of work hardening by successive cold working operations. Basically, work hardening occurs by converting the original grain shape into deformed, elongated grains by rolling or other cold working procedures. This grain shape change is illustrated schematically in Fig. 1. In this case, a copper zinc alloy is subjected to 60% reduction by cold rolling. The Reprinted from Practical Heat Treating, by Howard E. Boyer, copyright Ó 1984, American Society for Metals, Metals Park, Ohio. change in grain shape is evident. In practice, this much reduction in one pass would be rare, but the end result is essentially the same regardless of the number of passes. In this example, hardness of the alloy was originally 78 HRB, but changed to 131 HRB after cold reduction. This amount of hardness increase is typical of many copper alloys, most of which are very high in response to work hardening. Annealing of Nonferrous Metals and Alloys Most nonferrous alloys that have become hardened by cold work can be essentially restored to their original grain structure by annealing, during which process recrystallization occurs. This process is closely related to process annealing of low-carbon steels, which includes a certain amount of resulting grain growth that can be controlled to a great extent by annealing time and temperature. A typical example of the effects of annealing temperature on hardness (diamond pyramid or Vickers) of pure copper and a copper zinc alloy is presented in Fig. 2. Several facts are evident: The copper zinc alloy work hardens to a higher degree than pure copper. The effects of annealing are evident at a much lower temperature for pure copper compared to its companion alloy. Time at temperature has far less effect than temperature. Hardness of the pure metal and the alloy are nearly equal when near full annealing is accomplished at approximately 1110 F (600 C).
2 Metallogr. Microstruct. Anal. (2013) 2: same way as steels when subjected to heating and cooling treatments. At one time, technologists thought that ancient civilizations had developed a method for hardening copper alloys that had become a lost art. Copper articles removed from tombs showed a relatively high degree of hardness. However, it was proved that the impurities in these copper articles were responsible for their hardness. This hardness had evidently developed over a period of centuries by the precipitation mechanism rather than intentionally induced by the people who made them. Solubility and Insolubility Fig. 1 Schematic presentation of cold rolling a copper zinc alloy (60% reduction). Hardness was 78 HRB before reduction, which increased to 131 HRB after reduction. Source Heat Treatment, Structure and Properties of Nonferrous Alloys, p 22, 1982 In many instances, two or more metals, alloyed above their melting temperature, are completely soluble in each other, which continues through the solid solution range. For example, copper and tin alloy readily to form an entire family of bronzes. For these alloys, the solid solutions that form at elevated temperature remain completely stable at room temperature or below. Such an alloy, therefore, can be hardened only by cold working. On the other hand, many alloys contain phases or constituents that are readily soluble at elevated temperature, but are far less soluble or insoluble at room temperature, which is the basic requirement for hardening by heat treatment. General Heat Treating Procedures Fig. 2 Hardness as a function of annealing temperature for pure copper and a Cu 5Zn alloy, using three different annealing times. Both materials were originally cold rolled at 75 F (25 C) to a 60% reduction in thickness. Source Heat Treatment, Structure and Properties of Nonferrous Alloys, p 29, 1982 Figure 2 is presented as a simple example of recrystallization annealing. Each of the many nonferrous metals and metal alloy combinations has unique annealing characteristics which produce a unique graph of data. In many instances, adjustment may be required in the annealing time and/or temperature to attain desired grain size. Basic Requirements for Hardening by Heat Treatment As stated above, practically all nonferrous alloys respond readily to annealing treatments, but only a relatively small portion of the total number respond significantly to hardening by heat treatment. With the exception of titanium, common high-use aluminum, copper, and magnesium alloys, are not allotropic; thus, they do not respond in the Alloys with the characteristics described above are hardenable at least to some degree. The metallurgical principles responsible for this phenomenon are the same (or at least closely related) for all of the nonferrous alloys. Likewise, methods of processing are basically the same. However, temperature and time cycles cover a wide range, depending not only on alloy composition but also on whether the alloy is in the wrought or cast condition. As a rule, the highest possible increase in mechanical properties for a given alloy is accomplished in two distinct heating operations. First, the alloy is heated to a temperature just below (say at least 50 F or28 C) its solidus (beginning of melting) temperature. Holding time at temperature depends on the solubility of the various phases and whether the alloy is wrought or cast. It must be considered that the primary purpose of this operation is to affect a solid homogeneous solution of all phases. Consequently, this part of the operation is commonly known as solution treating or homogenizing. Because the structures of castings are relatively heterogeneous, a much longer time (at least twice as long) is required at the solution treating temperature compared to a wrought product of similar composition.
3 192 Metallogr. Microstruct. Anal. (2013) 2: Cooling From the Solutionizing Temperature After solid solution has been attained, the alloy is cooled as quickly as possible to room temperature (most often by water quenching) to arrest the structure obtained by heating. The required cooling rate is more critical for some alloys than for others. In addition, section thickness markedly affects cooling rate; still air is sometimes adequate. At this stage, the alloy is in the solution treated condition and, in most cases, is fully annealed (usually as soft as it can be made). However, the alloy is in an unstable condition because the phase or phases that possess a low degree of solubility at room temperature are virtually all dissolved. Aging (Precipitation Hardening) As soon as room temperature is reached, these phases start to precipitate out of solid solution in the form of fine particles within the crystals and at the grain boundaries. At one time, these particles were considered as submicroscopic, but the use of the electron microscope has changed this. In most alloys, precipitation occurs very slowly at room temperature and is even more sluggish at lower temperatures. In fact, this action in most alloys can be completely arrested by lowering to subzero temperatures. However, if the temperature of the solution treated alloy is raised, the action is greatly increased and can be completed in a relatively short time. Aging Cycles The precipitation or dispersion of fine particles tends to key the crystals together at their slip planes so that they are more resistant to deformation; thus, the alloy is stronger, harder, and less ductile. For each alloy, there is an optimum time and temperature. For the majority of nonferrous alloys, this is from about F ( C), although some alloys require higher aging temperatures. As is true for most heat treating operations, precipitation is a function of time and temperature. For example, a specific alloy might assume its maximum strength by aging for 5 h at 325 F (165 C), Overaging in either time or temperature is highly detrimental and decreases strength of the alloy. Specific Alloy Systems When precipitation hardening mechanisms are discussed, one is usually referring to nonferrous metals, although there are some iron-based alloys that are hardened by the precipitation mechanisms. Compositions and typical uses of some well-known alloys of aluminum, copper, magnesium, and nickel that respond readily to precipitation hardening are given in Table 1. The above discussion has, thus far, been quite general. We shall now take two commercially important alloys-one from the aluminum copper system and one from the copper beryllium system-and demonstrate more clearly the mechanism involved in solution treating and aging. As previously stated, time and temperature cycles vary greatly for different alloys, but the principles are basically the same for all precipitation hardening. To accomplish this, it is necessary to use phase diagrams. Aluminum Copper Alloys The first example that demonstrates the conditions which must exist for precipitation hardening is the partial aluminum copper phase diagram presented in Fig. 3. In this phase diagram, percent copper is plotted on the horizontal axis, and temperature is plotted on the vertical axis. The left side of the diagram (up to about 4.5% Cu) is the significant part of the diagram for showing the mechanisms of solution and aging. First, note that there is terminal solid solution (denoted as Al) on the left of the diagram (shaded area). The curved line ABC shows the maximum solid solubility of copper in aluminum for the temperature range of F ( C). The horizontal line at 1018 F (550 C) is the eutectic temperature. If the copper content is greater than that shown by line AB, the solid aluminum is saturated with copper and a new phase, CuAl 2, appears. Therefore, when aluminum containing about 4.5% Cu is heated to around 1000 F (540 C), it becomes a singlephase stable alloy at that temperature. Because of the similarity in size of the copper and aluminum atoms, the alloying is hardening by substitution (trading atoms from their lattice position) rather than by interstitial alloying. Thus, at various points in the aluminum lattice, copper atoms are substituted for aluminum atoms. When the alloy is quenched in water (or otherwise quickly cooled), there is insufficient time for the copper to precipitate as CuAl 2. According to Fig. 3, copper at room temperature is nearly insoluble in aluminum (shown as less than 1.0%). At this point, the alloy is in an unstable condition. Aging Under these very unstable conditions, some precipitation of CuAl 2 occurs at room temperature. This can be checked by
4 Metallogr. Microstruct. Anal. (2013) 2: Table 1 Precipitation hardenable alloys Source Metals Engineering Institute Course 1, Lesson 12, American Society for Metals, p 2, 1977 Alloy type Principal alloying elements (%) Typical uses Aluminum-based alloys 2014 (formerly 14S) 4.4 Cu, 0.8 Si, 0.8 Mn, 0.4 Mg Forged aircraft fittings, aluminum structures 2024 (formerly 24S) 4.5 Cu, 1.5 Mg, 0.6 Mn High-strength forgings, rivets, and structures 6061 (formerly 61S) 1 Mg, 0.6 Si, 0.25 Cu, 0.25 Cr Furniture, vacuum cleaners, canoes, and corrosion-resistant applications (used in ASM s geodesic dome) 7075 (formerly 75S) 5.5 Zn, 2.5 Mg, 1.5 Cu, 0.3 Cr Strong aluminum alloy; used in aircraft structures Copper-based alloys Beryllium bronze (beryllium copper) 1.9 Be, 0.2 Co or Ni Surgical instruments, electrical contacts, non-sparking tools, springs, nuts, gears, and other heavy duty applications 10 Al, 1 Fe Aluminum bronze Magnesium-based alloys AM100A 10 Al, 0.1 Mn Tough, leakproof sand castings AZ80A 8.5 Al, 0.5 Zn, 0.15 Mn min Extruded products and press forgings Nickel-based alloys Rene C, 19 Cr, 10 Co, 10 Mo, 3 Ti, 1.5 Al, 1.5 Fe, B Inconel 700 Udimet C, 15 Cr, 30 Co, 3 Mo, 2.2 Ti, 3.2 Al, 1 Fe 0.1 C, 19 Cr, 19 Co, 4 Mo, 3 Ti, 2.9 Al, 4 Fe (max.), B trace High temperature applications where strength is very important (up to about 1800 F) intervals. In a matter of hours, the alloy will register an increase in hardness caused by precipitation of CuAl 2, particles. The rate of hardness at room temperature, however, gradually diminishes, and after a time (say a few days), action practically ceases. However, if the as-quenched alloy is heated to about 340 F (1700 C) for several hours, the copper atoms regain enough mobility to effect the optimum amount of precipitation. Therefore, maximum attainable strength for the specific alloy is developed quickly by this artificial aging (purposely heating above room temperature). Overaging Fig. 3 Part of the aluminum copper phase diagram. The kappa phase, bounded by ABC, is a solid solution of copper in aluminum; CuAl 2 precipitates from this phase on slow cooling or on aging after solution treatment. Source Metals Engineering Institute Course 1, Lesson 12, American Society for Metals, p 3, 1977 first measuring the hardness in the as-quenched condition (essentially as soft as the alloy can be made), then continuing to take hardness measurements at regular There is an optimum time and temperature for aging of any specific alloy. When overaging takes place in terms of either time or temperature, or both there is a rapid drop in hardness. This is clearly shown in Fig. 4. It is also obvious from Fig. 4 that a fair-sized area exists that shows maximum hardness (zone 2), which indicates that there is some variation in the time temperature cycles. Changes in microstructure also are included in Fig. 4. Fine particles are precipitated in zone 2, whereas coarse particles (over precipitation) are shown within the grains in zone 3, where a definite decrease in hardness exists.
5 194 Metallogr. Microstruct. Anal. (2013) 2: Copper Beryllium Alloys Copper beryllium alloys hold a unique position among all other engineering alloys that are in use today. Copper by itself is used extensively throughout the electrical industry because it conducts electric current better than any other metal (excluding silver). Its resistance to the flow of current is low. By itself, however, copper does not have a great deal of strength. It is too soft to use in most structural applications. To impart some strength to copper, other elements are alloyed with it. One of the more potent of these is beryllium. The alloys of copper containing beryllium are among the strongest known of the copper alloy family. This high strength combined with good electrical conductivity makes copper beryllium alloys (also known as beryllium bronze or beryllium copper) particularly suited for electrical applications, as in contacts and relays which must open and shut a great number of times. Often these switches must open and close many times each minute, and during years of continuous service, they may be stressed a billion times or more. Beryllium bronze is highly suited for applications of this type. The same part may also serve as a structural member in the actual relay to hold it together and to support other parts. Heat treated copper beryllium alloys also have been used extensively in aircraft and aerospace applications. Phase Diagrams A partial copper beryllium phase diagram is presented in Fig. 5. This diagram can be interpreted in much the same manner as the aluminum copper system in Fig. 3. Figure 5 only shows beryllium contents up to 10%. The remainder of the phase diagram is not included because there are no commercial copper-based alloys in use with beryllium content above 2 %. Alloys with about 2% Be are used where high strength is required. A % Be alloy is used where high electrical conductivity is the main objective. However, to get good aging response, about 2% Ni or Co must be added to such an alloy. This phase diagram for the copper beryllium system is slightly more complex than those presented previously, and for that reason we will not discuss it here in any detail. The important feature to note is the all-important decreasing solubility of beryllium in the alpha (a) phase with decreasing temperature (large shaded area on the left of Fig. 5). The precipitation process in the copper beryllium alloy system is complicated by the beta phase changing into gamma. However, for the alloy under discussion the reader is interested only in the left portion of the phase diagram. Note that the primary requirement for precipitation hardening has been met; that is, beryllium has a very low solubility in copper at low temperatures and a relatively high solubility at elevated temperatures. Solution Treating and Aging In considering heat treatment, the shape of the hardness versus aging time curves for alloys with varying amounts Fig. 4 Schematic aging curve and microstructure. At a given aging temperature, the hardness of aluminum copper alloys increases to a maximum, then drops off. Source Metals Engineering Institute Course 1, Lesson 12, American Society for Metals, p 4, 1977 Fig. 5 Beryllium copper phase diagram. The alpha phase holds about 1.55% Be at 1121 F (605 C) and about 2.7% at 1590 F (865 C). Decreasing solubility of the beryllium causes precipitation of a hard beryllium copper phase on slow cooling or on aging after solution treatment. Source Metals Engineering Institute Course 1, Lesson 12, American Society for Metals, p 10, 1977
6 Metallogr. Microstruct. Anal. (2013) 2: hardening. The atoms of the parent lattice are displaced in making an adjustment. As a result of the shifting of position, the hardness of the alloy increases. A similar but less intensely stressed condition results in solid solution hardening. When beryllium atoms are present in the copper lattice, the copper atoms are forced to move slightly out of their normal position to accommodate the somewhat different size of the beryllium atom. This accommodation or slight shifting in position gives rise to a moderate increase in hardness. When more beryllium atoms are present, then more copper atoms have to shift. The result is a higher hardness as the number of beryllium atoms increases. Attaining Maximum Hardness Fig. 6 Precipitation-hardening curves of beryllium copper binary alloys. As the percentage of beryllium increases, the aging time required to reach maximum hardness is shortened, and the maximum hardness is increased. These alloys were quenched from 1470 F (800 C) and aged at 660 F (350 C) for the times shown. Source Metals Engineering Institute Course 1, Lesson 12, American Society for Metals, p 11, 1977 of beryllium should be considered. Figure 6 shows the aging curves for several copper beryllium alloys containing from 0.77 to 4.0% Be. These alloys were all solution treated at 1470 F (800 C) and aged at 660 F (350 C) for various lengths of time, as shown in Fig. 6. Note that an alloy containing as little as 0.77% Be does not harden as a result of aging. However, when the beryllium content is raised to 1.32%, a significant hardness increase takes place after 16 h. By increasing the beryllium content to 1.82%, a great deal of hardening takes place after 4 h, and the hardness stays at essentially the same level for the duration of the aging period. A beryllium content of 2.39% raises the peak hardness attained for this alloy. By increasing the beryllium content to 4%, still higher maximum hardnesses can be attained (Fig. 6). Several interesting observations can be made from examining Fig. 6. First, note that at zero aging time (the solution treated condition), alloys with higher beryllium content are harder. This is known as solid solution As the beryllium content is increased up to 2.39%, the time required to reach the maximum hardness decreases. Thus, aging for 36 h does not allow time enough to produce maximum hardness in a 1.32% Be alloy. With 1.82% Be, however, the maximum hardness occurs after approximately 5 h. With 2.39% Be or more, the maximum hardness occurs after only 1 h. It can also be seen from this diagram that by increasing the beryllium content above 2.39%, the rate of aging is not significantly increased. The 3.31 and 4% Be alloys reach a maximum hardness at about the same time as the 2.39% alloy. By looking at the phase diagram of the beryllium copper alloy system, the reason for this can be seen. The maximum solid solubility of beryllium in copper is just about 2.7% (at a temperature of 1590 F, or 865 C). Thus, the 3.31% alloy contains more than the maximum amount of beryllium that can be dissolved in copper. This means that the increased hardness of the 3.31 and 4% alloys is not due to any additional aging effects but is simply caused by the presence of undissolved beta phase, as may be predicted from the phase diagram. This increase in hardness on account of undissolved precipitate is known as dispersion hardening. The undissolved precipitate is harder than the matrix surrounding it, and the final hardness of the mixture depends on how much undissolved precipitate is present, as well as its manner of distribution.